#------------------------------------------------------------------------------
#$Date: 2016-03-26 02:00:26 +0200 (Sat, 26 Mar 2016) $
#$Revision: 180118 $
#$URL: svn://www.crystallography.net/cod/cif/7/10/16/7101638.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7101638
loop_
_publ_author_name
'Khatua, Snehadrinarayan'
'Roy, Debesh R'
'Chattaraj, Pratim K'
'Bhattacharjee, Manish'
_publ_section_title
;
 Synthesis and structure of 1-D Na6 cluster chain with short Na-Na
 distance: organic like aromaticity in inorganic metal cluster.
;
_journal_issue                   2
_journal_name_full
'Chemical communications (Cambridge, England)'
_journal_page_first              135
_journal_page_last               137
_journal_paper_doi               10.1039/b611693k
_journal_year                    2006
_chemical_formula_sum            'C4 H9 Mo N Na2 O9'
_chemical_formula_weight         357.04
_chemical_name_systematic
;
?
;
_space_group_IT_number           12
_symmetry_cell_setting           monoclinic
_symmetry_Int_Tables_number      12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 99.622(12)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   13.538(5)
_cell_length_b                   14.980(3)
_cell_length_c                   5.438(2)
_cell_measurement_reflns_used    25
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      13
_cell_measurement_theta_min      9
_cell_volume                     1087.4(6)
_computing_cell_refinement       'CAD4 Express (Enraf Nonius, 1994)'
_computing_data_collection       'CAD4 Express (Enraf Nonius, 1994)'
_computing_data_reduction        'XCAD4 (Harms & Wocadlo, 1995)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXL-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  CAD4
_diffrn_measurement_method       /w-scan
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0266
_diffrn_reflns_av_sigmaI/netI    0.0065
_diffrn_reflns_limit_h_max       16
_diffrn_reflns_limit_h_min       0
_diffrn_reflns_limit_k_max       17
_diffrn_reflns_limit_k_min       0
_diffrn_reflns_limit_l_max       6
_diffrn_reflns_limit_l_min       -6
_diffrn_reflns_number            1039
_diffrn_reflns_theta_full        24.94
_diffrn_reflns_theta_max         24.94
_diffrn_reflns_theta_min         2.04
_diffrn_standards_decay_%        0
_diffrn_standards_interval_time  60
_diffrn_standards_number         25
_exptl_absorpt_coefficient_mu    1.323
_exptl_absorpt_correction_type   none
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    2.181
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             704
_exptl_crystal_size_max          0.20
_exptl_crystal_size_mid          0.20
_exptl_crystal_size_min          0.10
_refine_diff_density_max         1.134
_refine_diff_density_min         -1.572
_refine_diff_density_rms         0.169
_refine_ls_extinction_coef       0.0248(16)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.047
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     95
_refine_ls_number_reflns         997
_refine_ls_number_restraints     3
_refine_ls_restrained_S_all      1.047
_refine_ls_R_factor_all          0.0304
_refine_ls_R_factor_gt           0.0302
_refine_ls_shift/su_max          0.015
_refine_ls_shift/su_mean         0.001
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0632P)²+3.9778P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0822
_refine_ls_wR_factor_ref         0.0823
_reflns_number_gt                991
_reflns_number_total             997
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            b611693k.txt
_cod_data_source_block           mbsnk001
_cod_depositor_comments
;
The following automatic conversions were performed:
'_symmetry_cell_setting' value 'Monoclinic' changed to 'monoclinic'
according to '/home/saulius/struct/CIF-dictionaries/cif_core.dic'
dictionary named 'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_enum 1527 2010-12-29 10:47:43Z saulius 
;
_cod_original_sg_symbol_H-M      C2/m
_cod_database_code               7101638
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z'
'-x, -y, -z'
'x, -y, z'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
C1 C 0.8364(3) 0.8779(2) 0.1274(6) 0.0205(7) Uani 1 1 d .
C2 C 0.8354(3) 0.9171(3) -0.1303(7) 0.0296(9) Uani 1 1 d .
H2A H 0.9037 0.9294 -0.1527 0.036 Uiso 1 1 calc R
H2B H 0.8076 0.8736 -0.2548 0.036 Uiso 1 1 calc R
N1 N 0.7764(3) 1.0000 -0.1704(7) 0.0163(8) Uani 1 2 d S
H1N H 0.739(7) 1.0000 -0.308(18) 0.07(3) Uiso 1 2 d S
O1 O 0.6099(2) 1.0000 0.3604(6) 0.0197(7) Uani 1 2 d S
O2 O 0.59753(18) 0.90830(16) -0.0946(4) 0.0209(5) Uani 1 1 d .
O3 O 0.77146(18) 0.90712(17) 0.2503(4) 0.0221(5) Uani 1 1 d .
O4 O 0.8965(2) 0.8176(2) 0.1971(5) 0.0372(7) Uani 1 1 d .
O5W O 0.6089(2) 0.78458(17) 0.3850(5) 0.0270(6) Uani 1 1 d D
H5WA H 0.622(4) 0.751(3) 0.517(7) 0.058(16) Uiso 1 1 d D
H5WB H 0.664(2) 0.813(3) 0.397(10) 0.051(15) Uiso 1 1 d D
Mo1 Mo 0.65208(2) 1.0000 0.07234(6) 0.0125(2) Uani 1 2 d S
Na1 Na 0.5000 0.89733(12) 0.5000 0.0203(4) Uani 1 2 d SD
Na2 Na 0.5000 0.77580(13) 0.0000 0.0217(4) Uani 1 2 d S
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O4 C1 O3 124.8(3) . .
O4 C1 C2 118.1(3) . .
O3 C1 C2 116.9(3) . .
N1 C2 C1 112.6(3) . .
N1 C2 H2A 109.1 . .
C1 C2 H2A 109.1 . .
N1 C2 H2B 109.1 . .
C1 C2 H2B 109.1 . .
H2A C2 H2B 107.8 . .
C2 N1 C2 115.0(4) 6_575 .
C2 N1 Mo1 110.2(2) 6_575 .
C2 N1 Mo1 110.2(2) . .
C2 N1 H1N 112(3) 6_575 .
C2 N1 H1N 112(3) . .
Mo1 N1 H1N 97(6) . .
O1 Na1 O1 98.33(12) . 5_676
O1 Na1 O2 88.33(10) . 1_556
O1 Na1 O2 86.49(11) 5_676 1_556
O1 Na1 O2 86.49(11) . 2_655
O1 Na1 O2 88.33(10) 5_676 2_655
O2 Na1 O2 172.08(15) 1_556 2_655
O1 Na1 O5W 175.19(10) . 2_656
O1 Na1 O5W 85.78(8) 5_676 2_656
O2 Na1 O5W 94.44(9) 1_556 2_656
O2 Na1 O5W 91.16(9) 2_655 2_656
O1 Na1 O5W 85.78(8) . .
O1 Na1 O5W 175.19(10) 5_676 .
O2 Na1 O5W 91.16(9) 1_556 .
O2 Na1 O5W 94.44(9) 2_655 .
O5W Na1 O5W 90.22(14) 2_656 .
O1 Na1 Na1 49.17(6) . 5_676
O1 Na1 Na1 49.17(6) 5_676 5_676
O2 Na1 Na1 86.04(7) 1_556 5_676
O2 Na1 Na1 86.04(7) 2_655 5_676
O5W Na1 Na1 134.89(7) 2_656 5_676
O5W Na1 Na1 134.89(7) . 5_676
O1 Na1 Na2 90.45(7) . .
O1 Na1 Na2 136.04(8) 5_676 .
O2 Na1 Na2 137.01(8) 1_556 .
O2 Na1 Na2 49.11(6) 2_655 .
O5W Na1 Na2 84.84(8) 2_656 .
O5W Na1 Na2 45.94(7) . .
Na1 Na1 Na2 123.81(4) 5_676 .
O1 Na1 Na2 136.04(8) . 1_556
O1 Na1 Na2 90.45(7) 5_676 1_556
O2 Na1 Na2 49.11(6) 1_556 1_556
O2 Na1 Na2 137.01(8) 2_655 1_556
O5W Na1 Na2 45.94(7) 2_656 1_556
O5W Na1 Na2 84.84(8) . 1_556
Na1 Na1 Na2 123.81(4) 5_676 1_556
Na2 Na1 Na2 112.39(8) . 1_556
O1 Na1 Mo1 112.37(8) . 5_676
O1 Na1 Mo1 22.23(7) 5_676 5_676
O2 Na1 Mo1 70.66(7) 1_556 5_676
O2 Na1 Mo1 105.88(7) 2_655 5_676
O5W Na1 Mo1 72.32(7) 2_656 5_676
O5W Na1 Mo1 153.14(7) . 5_676
Na1 Na1 Mo1 65.36(3) 5_676 5_676
Na2 Na1 Mo1 146.426(19) . 5_676
Na2 Na1 Mo1 68.33(3) 1_556 5_676
O1 Na1 Mo1 22.23(7) . .
O1 Na1 Mo1 112.37(8) 5_676 .
O2 Na1 Mo1 105.88(7) 1_556 .
O2 Na1 Mo1 70.66(7) 2_655 .
O5W Na1 Mo1 153.14(7) 2_656 .
O5W Na1 Mo1 72.32(7) . .
Na1 Na1 Mo1 65.36(3) 5_676 .
Na2 Na1 Mo1 68.33(3) . .
Na2 Na1 Mo1 146.426(19) 1_556 .
Mo1 Na1 Mo1 130.73(5) 5_676 .
O5W Na2 O5W 173.59(16) 2_655 .
O5W Na2 O4 96.07(10) 2_655 8_465
O5W Na2 O4 87.74(10) . 8_465
O5W Na2 O4 87.74(10) 2_655 7_665
O5W Na2 O4 96.07(10) . 7_665
O4 Na2 O4 107.30(17) 8_465 7_665
O5W Na2 O2 92.68(10) 2_655 .
O5W Na2 O2 82.18(9) . .
O4 Na2 O2 160.69(10) 8_465 .
O4 Na2 O2 90.18(10) 7_665 .
O5W Na2 O2 82.18(9) 2_655 2_655
O5W Na2 O2 92.68(10) . 2_655
O4 Na2 O2 90.18(10) 8_465 2_655
O4 Na2 O2 160.69(10) 7_665 2_655
O2 Na2 O2 73.98(13) . 2_655
O5W Na2 Na1 128.37(9) 2_655 .
O5W Na2 Na1 46.92(7) . .
O4 Na2 Na1 82.53(7) 8_465 .
O4 Na2 Na1 142.14(8) 7_665 .
O2 Na2 Na1 78.55(7) . .
O2 Na2 Na1 46.35(6) 2_655 .
O5W Na2 Na1 46.92(7) 2_655 1_554
O5W Na2 Na1 128.37(9) . 1_554
O4 Na2 Na1 142.14(8) 8_465 1_554
O4 Na2 Na1 82.53(7) 7_665 1_554
O2 Na2 Na1 46.35(6) . 1_554
O2 Na2 Na1 78.55(7) 2_655 1_554
Na1 Na2 Na1 112.39(8) . 1_554
C1 O3 Mo1 120.2(2) . .
O2 Mo1 O2 104.15(16) . 6_575
O2 Mo1 O1 107.01(10) . .
O2 Mo1 O1 107.01(10) 6_575 .
O2 Mo1 O3 158.90(11) . 6_575
O2 Mo1 O3 86.99(10) 6_575 6_575
O1 Mo1 O3 86.15(11) . 6_575
O2 Mo1 O3 86.99(10) . .
O2 Mo1 O3 158.90(11) 6_575 .
O1 Mo1 O3 86.15(11) . .
O3 Mo1 O3 77.31(14) 6_575 .
O2 Mo1 N1 89.31(10) . .
O2 Mo1 N1 89.31(10) 6_575 .
O1 Mo1 N1 152.69(15) . .
O3 Mo1 N1 72.71(10) 6_575 .
O3 Mo1 N1 72.71(10) . .
O2 Mo1 Na1 76.54(8) . .
O2 Mo1 Na1 115.14(8) 6_575 .
O1 Mo1 Na1 30.47(7) . .
O3 Mo1 Na1 115.29(6) 6_575 .
O3 Mo1 Na1 84.63(7) . .
N1 Mo1 Na1 153.94(4) . .
O2 Mo1 Na1 115.14(8) . 5_676
O2 Mo1 Na1 76.54(8) 6_575 5_676
O1 Mo1 Na1 30.47(7) . 5_676
O3 Mo1 Na1 84.63(7) 6_575 5_676
O3 Mo1 Na1 115.29(6) . 5_676
N1 Mo1 Na1 153.94(4) . 5_676
Na1 Mo1 Na1 49.27(5) . 5_676
Mo1 O1 Na1 127.29(11) . .
Mo1 O1 Na1 127.29(11) . 5_676
Na1 O1 Na1 81.67(12) . 5_676
Mo1 O2 Na1 131.23(13) . 1_554
Mo1 O2 Na2 135.71(12) . .
Na1 O2 Na2 84.54(8) 1_554 .
C1 O4 Na2 134.9(2) . 7_665
Na2 O5W Na1 87.14(10) . .
Na2 O5W H5WA 136(4) . .
Na1 O5W H5WA 104(3) . .
Na2 O5W H5WB 120(4) . .
Na1 O5W H5WB 102(4) . .
H5WA O5W H5WB 99(5) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
C1 O4 1.233(4) .
C1 O3 1.268(4) .
C1 C2 1.517(5) .
C2 N1 1.472(4) .
C2 H2A 0.9700 .
C2 H2B 0.9700 .
N1 C2 1.472(4) 6_575
N1 Mo1 2.306(4) .
N1 H1N 0.83(10) .
Na1 O1 2.352(3) .
Na1 O1 2.352(3) 5_676
Na1 O2 2.378(2) 1_556
Na1 O2 2.378(2) 2_655
Na1 O5W 2.393(3) 2_656
Na1 O5W 2.393(3) .
Na1 Na1 3.076(4) 5_676
Na1 Na2 3.2723(17) .
Na1 Na2 3.2723(17) 1_556
Na1 Mo1 3.6897(12) 5_676
Na1 Mo1 3.6897(12) .
Na2 O5W 2.354(3) 2_655
Na2 O5W 2.354(3) .
Na2 O4 2.360(3) 8_465
Na2 O4 2.360(3) 7_665
Na2 O2 2.485(3) .
Na2 O2 2.485(3) 2_655
Na2 Na1 3.2723(17) 1_554
O3 Mo1 2.228(2) .
Mo1 O2 1.741(2) .
Mo1 O2 1.741(2) 6_575
Mo1 O1 1.755(3) .
Mo1 O3 2.228(2) 6_575
Mo1 Na1 3.6897(12) 5_676
O1 Na1 2.352(3) 5_676
O2 Na1 2.378(2) 1_554
O4 Na2 2.360(3) 7_665
O5W H5WA 0.87(2) .
O5W H5WB 0.86(2) .
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
O4 C1 C2 N1 -167.9(3) . .
O3 C1 C2 N1 15.4(5) . .
C1 C2 N1 C2 97.3(4) . 6_575
C1 C2 N1 Mo1 -27.9(4) . .
O1 Na1 Na2 O5W -90.56(13) . 2_655
O1 Na1 Na2 O5W 11.96(17) 5_676 2_655
O2 Na1 Na2 O5W -178.59(13) 1_556 2_655
O2 Na1 Na2 O5W -5.59(12) 2_655 2_655
O5W Na1 Na2 O5W 90.43(13) 2_656 2_655
O5W Na1 Na2 O5W -174.25(14) . 2_655
Na1 Na1 Na2 O5W -51.98(10) 5_676 2_655
Na2 Na1 Na2 O5W 128.02(10) 1_556 2_655
Mo1 Na1 Na2 O5W 43.86(17) 5_676 2_655
Mo1 Na1 Na2 O5W -88.28(11) . 2_655
O1 Na1 Na2 O5W 83.69(12) . .
O1 Na1 Na2 O5W -173.78(15) 5_676 .
O2 Na1 Na2 O5W -4.33(14) 1_556 .
O2 Na1 Na2 O5W 168.66(13) 2_655 .
O5W Na1 Na2 O5W -95.31(15) 2_656 .
Na1 Na1 Na2 O5W 122.28(10) 5_676 .
Na2 Na1 Na2 O5W -57.73(10) 1_556 .
Mo1 Na1 Na2 O5W -141.89(14) 5_676 .
Mo1 Na1 Na2 O5W 85.98(9) . .
O1 Na1 Na2 O4 177.60(11) . 8_465
O1 Na1 Na2 O4 -79.88(14) 5_676 8_465
O2 Na1 Na2 O4 89.57(14) 1_556 8_465
O2 Na1 Na2 O4 -97.43(12) 2_655 8_465
O5W Na1 Na2 O4 -1.41(11) 2_656 8_465
O5W Na1 Na2 O4 93.90(13) . 8_465
Na1 Na1 Na2 O4 -143.82(8) 5_676 8_465
Na2 Na1 Na2 O4 36.18(8) 1_556 8_465
Mo1 Na1 Na2 O4 -47.99(13) 5_676 8_465
Mo1 Na1 Na2 O4 179.88(9) . 8_465
O1 Na1 Na2 O4 68.93(17) . 7_665
O1 Na1 Na2 O4 171.45(16) 5_676 7_665
O2 Na1 Na2 O4 -19.1(2) 1_556 7_665
O2 Na1 Na2 O4 153.90(18) 2_655 7_665
O5W Na1 Na2 O4 -110.08(17) 2_656 7_665
O5W Na1 Na2 O4 -14.76(17) . 7_665
Na1 Na1 Na2 O4 107.51(15) 5_676 7_665
Na2 Na1 Na2 O4 -72.49(15) 1_556 7_665
Mo1 Na1 Na2 O4 -156.66(14) 5_676 7_665
Mo1 Na1 Na2 O4 71.21(15) . 7_665
O1 Na1 Na2 O2 -6.27(9) . .
O1 Na1 Na2 O2 96.25(12) 5_676 .
O2 Na1 Na2 O2 -94.30(13) 1_556 .
O2 Na1 Na2 O2 78.70(14) 2_655 .
O5W Na1 Na2 O2 174.72(9) 2_656 .
O5W Na1 Na2 O2 -89.96(11) . .
Na1 Na1 Na2 O2 32.31(6) 5_676 .
Na2 Na1 Na2 O2 -147.69(6) 1_556 .
Mo1 Na1 Na2 O2 128.15(11) 5_676 .
Mo1 Na1 Na2 O2 -3.99(6) . .
O1 Na1 Na2 O2 -84.97(12) . 2_655
O1 Na1 Na2 O2 17.55(13) 5_676 2_655
O2 Na1 Na2 O2 -173.00(14) 1_556 2_655
O5W Na1 Na2 O2 96.02(10) 2_656 2_655
O5W Na1 Na2 O2 -168.66(13) . 2_655
Na1 Na1 Na2 O2 -46.39(8) 5_676 2_655
Na2 Na1 Na2 O2 133.61(8) 1_556 2_655
Mo1 Na1 Na2 O2 49.45(12) 5_676 2_655
Mo1 Na1 Na2 O2 -82.69(9) . 2_655
O1 Na1 Na2 Na1 -38.58(7) . 1_554
O1 Na1 Na2 Na1 63.94(11) 5_676 1_554
O2 Na1 Na2 Na1 -126.61(11) 1_556 1_554
O2 Na1 Na2 Na1 46.39(8) 2_655 1_554
O5W Na1 Na2 Na1 142.41(7) 2_656 1_554
O5W Na1 Na2 Na1 -122.28(10) . 1_554
Na1 Na1 Na2 Na1 0.0 5_676 1_554
Na2 Na1 Na2 Na1 180.0 1_556 1_554
Mo1 Na1 Na2 Na1 95.83(9) 5_676 1_554
Mo1 Na1 Na2 Na1 -36.300(16) . 1_554
O4 C1 O3 Mo1 -169.7(3) . .
C2 C1 O3 Mo1 6.7(4) . .
C1 O3 Mo1 O2 73.2(3) . .
C1 O3 Mo1 O2 -49.8(4) . 6_575
C1 O3 Mo1 O1 -179.5(3) . .
C1 O3 Mo1 O3 -92.6(3) . 6_575
C1 O3 Mo1 N1 -17.0(2) . .
C1 O3 Mo1 Na1 149.9(3) . .
C1 O3 Mo1 Na1 -170.4(2) . 5_676
C2 N1 Mo1 O2 168.1(3) 6_575 .
C2 N1 Mo1 O2 -64.0(3) . .
C2 N1 Mo1 O2 64.0(3) 6_575 6_575
C2 N1 Mo1 O2 -168.1(3) . 6_575
C2 N1 Mo1 O1 -63.9(3) 6_575 .
C2 N1 Mo1 O1 63.9(3) . .
C2 N1 Mo1 O3 -23.1(3) 6_575 6_575
C2 N1 Mo1 O3 104.8(3) . 6_575
C2 N1 Mo1 O3 -104.8(3) 6_575 .
C2 N1 Mo1 O3 23.1(3) . .
C2 N1 Mo1 Na1 -135.54(19) 6_575 .
C2 N1 Mo1 Na1 -7.7(4) . .
C2 N1 Mo1 Na1 7.7(4) 6_575 5_676
C2 N1 Mo1 Na1 135.54(19) . 5_676
O1 Na1 Mo1 O2 179.7(2) . .
O1 Na1 Mo1 O2 -126.64(12) 5_676 .
O2 Na1 Mo1 O2 140.60(15) 1_556 .
O2 Na1 Mo1 O2 -46.88(9) 2_655 .
O5W Na1 Mo1 O2 2.90(18) 2_656 .
O5W Na1 Mo1 O2 54.53(11) . .
Na1 Na1 Mo1 O2 -141.49(8) 5_676 .
Na2 Na1 Mo1 O2 5.74(9) . .
Na2 Na1 Mo1 O2 103.93(13) 1_556 .
Mo1 Na1 Mo1 O2 -141.49(8) 5_676 .
O1 Na1 Mo1 O2 -80.8(2) . 6_575
O1 Na1 Mo1 O2 -27.12(13) 5_676 6_575
O2 Na1 Mo1 O2 -119.89(8) 1_556 6_575
O2 Na1 Mo1 O2 52.63(14) 2_655 6_575
O5W Na1 Mo1 O2 102.41(19) 2_656 6_575
O5W Na1 Mo1 O2 154.05(11) . 6_575
Na1 Na1 Mo1 O2 -41.98(9) 5_676 6_575
Na2 Na1 Mo1 O2 105.26(9) . 6_575
Na2 Na1 Mo1 O2 -156.55(12) 1_556 6_575
Mo1 Na1 Mo1 O2 -41.98(9) 5_676 6_575
O1 Na1 Mo1 O1 53.7(3) 5_676 .
O2 Na1 Mo1 O1 -39.11(19) 1_556 .
O2 Na1 Mo1 O1 133.4(2) 2_655 .
O5W Na1 Mo1 O1 -176.8(3) 2_656 .
O5W Na1 Mo1 O1 -125.17(19) . .
Na1 Na1 Mo1 O1 38.80(18) 5_676 .
Na2 Na1 Mo1 O1 -173.96(18) . .
Na2 Na1 Mo1 O1 -75.77(19) 1_556 .
Mo1 Na1 Mo1 O1 38.80(18) 5_676 .
O1 Na1 Mo1 O3 18.3(2) . 6_575
O1 Na1 Mo1 O3 71.94(11) 5_676 6_575
O2 Na1 Mo1 O3 -20.82(11) 1_556 6_575
O2 Na1 Mo1 O3 151.70(10) 2_655 6_575
O5W Na1 Mo1 O3 -158.52(18) 2_656 6_575
O5W Na1 Mo1 O3 -106.88(10) . 6_575
Na1 Na1 Mo1 O3 57.09(8) 5_676 6_575
Na2 Na1 Mo1 O3 -155.68(8) . 6_575
Na2 Na1 Mo1 O3 -57.49(13) 1_556 6_575
Mo1 Na1 Mo1 O3 57.09(8) 5_676 6_575
O1 Na1 Mo1 O3 91.52(19) . .
O1 Na1 Mo1 O3 145.18(11) 5_676 .
O2 Na1 Mo1 O3 52.42(10) 1_556 .
O2 Na1 Mo1 O3 -135.06(10) 2_655 .
O5W Na1 Mo1 O3 -85.28(18) 2_656 .
O5W Na1 Mo1 O3 -33.65(9) . .
Na1 Na1 Mo1 O3 130.33(7) 5_676 .
Na2 Na1 Mo1 O3 -82.44(7) . .
Na2 Na1 Mo1 O3 15.75(12) 1_556 .
Mo1 Na1 Mo1 O3 130.33(7) 5_676 .
O1 Na1 Mo1 N1 120.9(3) . .
O1 Na1 Mo1 N1 174.5(2) 5_676 .
O2 Na1 Mo1 N1 81.8(2) 1_556 .
O2 Na1 Mo1 N1 -105.7(2) 2_655 .
O5W Na1 Mo1 N1 -55.9(3) 2_656 .
O5W Na1 Mo1 N1 -4.3(2) . .
Na1 Na1 Mo1 N1 159.7(2) 5_676 .
Na2 Na1 Mo1 N1 -53.1(2) . .
Na2 Na1 Mo1 N1 45.1(2) 1_556 .
Mo1 Na1 Mo1 N1 159.7(2) 5_676 .
O1 Na1 Mo1 Na1 -38.80(18) . 5_676
O1 Na1 Mo1 Na1 14.86(9) 5_676 5_676
O2 Na1 Mo1 Na1 -77.91(8) 1_556 5_676
O2 Na1 Mo1 Na1 94.61(7) 2_655 5_676
O5W Na1 Mo1 Na1 144.39(16) 2_656 5_676
O5W Na1 Mo1 Na1 -163.97(7) . 5_676
Na2 Na1 Mo1 Na1 147.24(2) . 5_676
Na2 Na1 Mo1 Na1 -114.58(10) 1_556 5_676
Mo1 Na1 Mo1 Na1 0.0 5_676 5_676
O2 Mo1 O1 Na1 -0.3(2) . .
O2 Mo1 O1 Na1 110.86(15) 6_575 .
O3 Mo1 O1 Na1 -163.48(17) 6_575 .
O3 Mo1 O1 Na1 -85.96(17) . .
N1 Mo1 O1 Na1 -124.72(16) . .
Na1 Mo1 O1 Na1 110.6(3) 5_676 .
O2 Mo1 O1 Na1 -110.86(15) . 5_676
O2 Mo1 O1 Na1 0.3(2) 6_575 5_676
O3 Mo1 O1 Na1 85.96(17) 6_575 5_676
O3 Mo1 O1 Na1 163.48(17) . 5_676
N1 Mo1 O1 Na1 124.72(16) . 5_676
Na1 Mo1 O1 Na1 -110.6(3) . 5_676
O1 Na1 O1 Mo1 -131.2(2) 5_676 .
O2 Na1 O1 Mo1 142.63(18) 1_556 .
O2 Na1 O1 Mo1 -43.37(18) 2_655 .
O5W Na1 O1 Mo1 51.35(17) . .
Na1 Na1 O1 Mo1 -131.2(2) 5_676 .
Na2 Na1 O1 Mo1 5.61(17) . .
Na2 Na1 O1 Mo1 129.45(16) 1_556 .
Mo1 Na1 O1 Mo1 -149.10(13) 5_676 .
O1 Na1 O1 Na1 0.0 5_676 5_676
O2 Na1 O1 Na1 -86.21(10) 1_556 5_676
O2 Na1 O1 Na1 87.79(10) 2_655 5_676
O5W Na1 O1 Na1 -177.49(10) . 5_676
Na2 Na1 O1 Na1 136.77(7) . 5_676
Na2 Na1 O1 Na1 -99.39(11) 1_556 5_676
Mo1 Na1 O1 Na1 -17.94(10) 5_676 5_676
Mo1 Na1 O1 Na1 131.2(2) . 5_676
O2 Mo1 O2 Na1 12.8(2) 6_575 1_554
O1 Mo1 O2 Na1 125.88(16) . 1_554
O3 Mo1 O2 Na1 -107.4(3) 6_575 1_554
O3 Mo1 O2 Na1 -149.08(16) . 1_554
N1 Mo1 O2 Na1 -76.36(17) . 1_554
Na1 Mo1 O2 Na1 125.72(16) . 1_554
Na1 Mo1 O2 Na1 94.31(15) 5_676 1_554
O2 Mo1 O2 Na2 -123.06(14) 6_575 .
O1 Mo1 O2 Na2 -9.9(2) . .
O3 Mo1 O2 Na2 116.8(2) 6_575 .
O3 Mo1 O2 Na2 75.10(18) . .
N1 Mo1 O2 Na2 147.82(19) . .
Na1 Mo1 O2 Na2 -10.10(15) . .
Na1 Mo1 O2 Na2 -41.5(2) 5_676 .
O5W Na2 O2 Mo1 139.97(18) 2_655 .
O5W Na2 O2 Mo1 -36.19(19) . .
O4 Na2 O2 Mo1 23.0(4) 8_465 .
O4 Na2 O2 Mo1 -132.29(19) 7_665 .
O2 Na2 O2 Mo1 58.89(15) 2_655 .
Na1 Na2 O2 Mo1 11.31(17) . .
Na1 Na2 O2 Mo1 148.2(2) 1_554 .
O5W Na2 O2 Na1 -8.27(9) 2_655 1_554
O5W Na2 O2 Na1 175.58(10) . 1_554
O4 Na2 O2 Na1 -125.2(3) 8_465 1_554
O4 Na2 O2 Na1 79.48(9) 7_665 1_554
O2 Na2 O2 Na1 -89.34(9) 2_655 1_554
Na1 Na2 O2 Na1 -136.92(8) . 1_554
O3 C1 O4 Na2 163.5(3) . 7_665
C2 C1 O4 Na2 -12.9(6) . 7_665
O4 Na2 O5W Na1 -81.89(11) 8_465 .
O4 Na2 O5W Na1 170.95(10) 7_665 .
O2 Na2 O5W Na1 81.61(9) . .
O2 Na2 O5W Na1 8.19(9) 2_655 .
Na1 Na2 O5W Na1 85.69(12) 1_554 .
O1 Na1 O5W Na2 -94.72(11) . .
O2 Na1 O5W Na2 177.05(10) 1_556 .
O2 Na1 O5W Na2 -8.57(10) 2_655 .
O5W Na1 O5W Na2 82.60(9) 2_656 .
Na1 Na1 O5W Na2 -97.40(9) 5_676 .
Na2 Na1 O5W Na2 128.29(9) 1_556 .
Mo1 Na1 O5W Na2 130.94(13) 5_676 .
Mo1 Na1 O5W Na2 -76.65(7) . .
